In situ Scanning Electron
Microscopy of Silicon Anode
Reactions in Lithium-Ion Batteries
during Charge/Discharge Processes
, Teruki Sano1
, Tetsuya Tsuda1
, Koichi Ui2
, Yoshifumi Oshima3
, Masashi Ishikawa4
, Masakazu Haruta5
, Takayuki Doi5
, Minoru Inaba5
A comprehensive understanding of the charge/discharge behaviour of high-capacity anode active materials, e.g., Si and Li, is essential for the design and development of next-generation
high-performance Li-based batteries. Here, we demonstrate the in situ scanning electron microscopy (in situ SEM) of Si anodes in a configuration analogous to actual lithium-ion batteries (LIBs) with an ionic liquid (IL) that is expected to be a functional LIB electrolyte in the future. We discovered that variations in the morphology of Si active materials during charge/discharge processes is strongly dependent on their size and shape. Even the diffusion of atomic Li into Si materials can be visualized using a back-scattering electron imaging technique. The electrode reactions were successfully recorded as video clips. This
in situ SEM technique can simultaneously provide useful data on, for example, morphological variations
and elemental distributions, as well as electrochemical data.
Silicon is one of the most appealing next-generation anode active materials for future lithium-ion batteries (LIBs) with outstanding theoretical capacities (e.g., 3579 mAh g−1 for Li15Si4) nearly an order of magnitude greater than that of a conventional graphite battery (372 mAh g−1)1,2. However, the dramatic volume change (up to approx-imately 300%) experienced during charging/discharging, i.e., alloying/dealloying with Li, often leads to severe pulverization and the subsequent loss of electrical contact. In many cases, these mechanical phenomena result in a fatal capacity drop. This is a barrier to the practical application of Si anodes. Silicon nanostructuring is regarded as an effective strategy to relieve mechanical stress2. Several promising configurations have been proposed, such as nanoparticles3,4, nanowires5, nanotubes6, thin films7,8, nano-hairy structures9, and Si thin flakes (synonym: Si LeafPowder
®)10,11. Of these, Si thin flakes are recognized as a well-balanced material because they can be readily stacked in layers without sacrificing the advantages associated with nanostructures; thus, they not only possess high, nanomaterial-like capacity and stable cyclabilities but also offer bulk-like tap density.
Ionic liquids (ILs), which are liquid salts at room temperature, have considerable potential as advanced electrolytes for LIBs owing to of their unique properties: wide electrochemical windows, negligible vapour pressures, nonflammability, and good thermal and electrochemical stability12,13. Several research groups have combined bis(fluorosulfonyl)amide (N(SO2F)2, FSA)-based ILs and Si anodes for the development of future LIB systems14–17. For example, Piper, et al. successfully combined these components into a LIB system17, which showed both remarkable capacity retention (> 75% after 500 cycles) and an unprecedented coulombic efficiency (99.97% for the first 200 cycles). In the past decade, analytical approaches for studying an electrode reaction in a LIB cell, e.g., X-ray diffraction (XRD)18,19, atomic force microscopy (AFM)20, nuclear magnetic resonance 1Department of Applied Chemistry, Graduate School of Engineering, Osaka University, 2-1 Yamada-oka, Suita, Osaka, 565-0871, Japan. 2Department of Frontier Materials and Function Engineering, Graduate School of Engineering, Iwate University, 4-3-5 Ueda, Morioka, Iwate, 020-8551, Japan. 3School of Materials Science, Japan Advanced Institute of Science and Technology, 1-1 Asahidai, Nomi, Ishikawa, 923-1292, Japan. 4Department of Chemistry and Materials Engineering, Kansai University, 3-3-35 Yamate-cho, Suita, Osaka, 564-8680, Japan. 5Department of Molecular Chemistry and Biochemistry, Doshisha University, 1-3 Tatara Miyakodani, Kyotanabe, Kyoto, 610-0321, Japan. Correspondence and requests for materials should be addressed to T.T. (email: ttsuda@ chem.eng.osaka-u.ac.jp) or S.K. (email: firstname.lastname@example.org)
received: 02 September 2016 accepted: 11 October 2016 Published: 26 October 2016
as the anode. The surface electric charge state of the Si active materials and an acetylene black (AB) conduction supporting agent was modified by adding citric acid to a dry acetone bath. This enabled the codeposition of Si and AB onto a copper mesh current collector31. The active materials, which had different shapes and sizes, were Si microparticles, Si nanoparticle aggregates, and Si thin flakes, as shown in Fig. 1a–c. As an example, Fig. 1d depicts a fabrication process for a binder-free Si thin flake electrode. The conceptual cell setup for the in situ SEM equip-ment used in this research is illustrated in Fig. 1e. The electrodes and separator were located, and their configura-tion was quite similar to that found in a typical LIB. A nonvolatile IL electrolyte—1-ethyl-3-methylimidazolium bis(fluorosulfonyl)amide ([C2 mim][FSA]) containing 1.0 mol L−1 lithium bis(trifluoromethanesulfonyl)amide (Li[TFSA])—was selected as the electrolyte for the cell32. A photograph of the assembled cell is shown in Supplementary Fig. 1a. Supplementary Fig. 1b is a digital microscope image of the Si microparticle electrode. This electrode is covered with the IL electrolyte. Thus, the electrochemical lithiation/delithiation reactions of the Si active materials proceed in the areas where the active materials encounter the electrolyte. However, the electrolyte should be a very thin layer (up to approximately 100 nm) to obtain a clear in situ SEM image of the Si anode33–35. Otherwise, only a smooth IL surface will be observed, as shown in Supplementary Fig. 1c.
Charge/discharge curves recorded at the Si microparticle anode are shown in Fig. 2a. At the 1st cycle, a sub-stantial irreversible capacity was identified. Similar behaviour has also been reported by other research groups, and its underlying reason has been investigated23,36,37. Figure 2b–d show SEM images displaying the morphology variation in the Si microparticles during the 1st charge/discharge process. Typical several particles are surrounded by yellow circles. After the 1st charge process, the Si particles expanded considerably because of the formation of lithiated Si (LixSi), but this expansion was not isotropic. This non-uniform expansion implies that lithiation
initiates at a point between the Si particles and the current collector. The lithiated Si microparticles shrank during the 1st discharge process and did not fully recover to their original size. Enlarged images obtained from a different area during the same cycle are shown in Fig. 2e–g. Several cracks appeared during the charge process. Tensile stress in the external surface of the lithiated section is known to increase as lithiation proceeds38,39. The stress in the outer layer triggers fracturing that is directly related to capacity loss. Most of the cracks became nearly invisi-ble as a result of shrinking back during the discharge process. Moreover, we succeeded in capturing this on video at the same place as Fig. 2e–g during the 2nd charge/discharge process (Movies 1 and 2 in the supplementary information). In Movie 1, severe volume expansion followed by a sudden reappearance of cracks was observed upon the 2nd charge process. Interestingly, the largest microparticle in the movie was moved by direct con-tact with a neighbouring small particle, and subsequently, the microparticle became electrochemically inactive, clearly indicating that it lost its electrical contact with the current collector (Movie 2). Two types of mechanical damage—fracturing of the Si microparticles and breakdown of the conductive network—resulting from the lithi-ation reaction were visually identified via in situ SEM. These types of damage mainly contribute to the enormous irreversible capacity observed in the first cycle, although other contributors should also be considered, such as solid-electrolyte interphase (SEI) formation resulting from the decomposition of the IL on the lithiated Si14,17,40.
We also observed the electrowetting behaviour of the IL electrolyte, which can be explained by the difference in the ion sizes of cations and anions41, during the charge process on an electron-microscopic scale. This informa-tion can be obtained only using this in situ technique. It will be useful informainforma-tion in designing the LIB cell with a bare minimum of the IL electrolyte. Compared to the in situ SEM image, the ex situ SEM image of the largest particle shown in Fig. 2g collected after rinsing the anode with diethyl carbonate (DEC) is completely different (Supplementary Fig. 2). Notably, the ex situ image includes artefacts that may arise during electrode recovery and rinsing. Therefore, in situ SEM is highly advantageous relative to ex situ observations.
For the Si nanoparticle aggregates, no cracks were identified during the 1st charge/discharge process (Fig. 3a–c). Most of the aggregates exhibited relatively isotropic volume expansion and shrinkage because the higher surface-to-volume ratio of the Si nanoparticle facilitates full lithiation. To quantify the lithiation behaviour of the Si nanoparticle aggregates, the volume variations (%) after the charge and discharge processes relatively to the initial volume—Vcharged/Vinitial and Vdischarged/Vinitial, respectively—were estimated. We assumed that the height of each aggregate is half the sum of its width (W) and length (L). To reduce the error, the volume calculation was applied only to near-spherical aggregates (L/W < 1.30). The statistical analysis revealed that most Si particles after the charge process approached the theoretical value for Li15Si4 formation, approximately 370% (74.9 Å3 for Li15Si4 per Si atom and 20.0 Å3 for crystalline Si)42,43, and obvious irreversible volume alteration was observed after the discharge (Fig. 3d). The relative frequency of Vdischarged/Vinitial peaked at a volume change of 150–200%. This is
attributable to the fact that dense packing of Si nanoparticle aggregates loosened upon electrochemical cycling and nanoscale pores were generated through clustering of vacancies left behind by lithium-ion stripping26.
According to Griffith’s fracture criterion, cracking should occur only if the stored strain energy exceeds the surface energy of the new surface with cracks2,38,39. This model is also applicable to Si particles. The stress-relief volume and surface energy resistance relevant to crack growth depend on the Si particle size38. Various studies have been conducted to elucidate the critical Si particle size without lithiation-driven fracturing38,39,44–46. The
Figure 1. Schematic drawings of the Si anode preparation process and an in situ SEM observation cell. (a–c)
SEM images of the Si active materials used in this study. The active materials were (a) Si microparticles, (b) Si nanoparticle aggregates, and (c) Si thin flakes. (d) Binder-free Si anode fabrication process via the electrophoretic deposition (EPD) method. Here, Si thin flakes were employed as the Si active material. (e) Illustration of a typical Li-ion battery system with a binder-free Si thin flake anode for in situ SEM.
Figure 2. In situ SEM images of a Si microparticle anode during the 1st charge/discharge process. (a) The
charge/discharge curves of a Si microparticle anode recorded in constant current and constant voltage (CC/CV) mode with cut-off voltages ranging between − 3.88 V and − 2.40 V (vs. LiCoO2). The CC rates for charge and discharge were 0.12 C. (b–g) In situ SEM images of the Si microparticles. (b,e) The initial state. (c,f) After the charge process. (d,g) After the discharge process.
Figure 3. In situ SEM images of a Si nanoparticle aggregate anode (Davg for aggregates: approximately
10 μm; Davg for nano-Si particles: approximately 100 nm) during the 1st charge/discharge process. The
charge/discharge conditions were 0.25 C (constant current mode) at cut-off voltages of − 3.88 V and − 2.40 V (vs. LiCoO2). (a–c) In situ SEM images of Si nanoparticle aggregates. (d) The relative frequencies as a function of the volume change in Si nanoparticle aggregates after (blue) the charge and (red) discharge processes relative to the initial volume.
critical particle sizes proposed to date range from hundreds of nanometres to 10 μ m. For example, Kalnaus et al., on the basis of both experimental evidence and theoretical prediction, reported that the probability of mechanical failure sharply increases if the particle radius exceeds the proposed range46. Our in situ SEM results are in good agreement with the model vaguely proposed by a number of research groups.
Figure 4a shows the charge/discharge curves of a Si thin flake anode measured in constant current/constant voltage (CC/CV) and CC modes for charging and discharging, respectively, with cut-off voltages ranging between − 3.88 V and − 2.40 V (vs. LiCoO2). As described below, the discharge capacity retention stabilized after several cycles, although the irreversible capacity clearly appeared during the 1st cycling, similar to other Si active mate-rials7,8,14,31. A series of SEM images captured from Movies 3 and 4 displaying the charge/discharge behaviour of a Si thin flake anode at the 3rd cycle are shown in Fig. 4b. As expected, the Si flakes expanded during charging. Surprisingly, however, two expansion processes were identified: a readily predictable flat-plate type expansion and a ribbon-type expansion (Fig. 4c). In the latter, the mechanical stress caused by the lithiation process appears to be spontaneously relieved by the flexible expansion. Indeed, we found no evidence of serious damage, e.g., fracturing and cracks, in the Si flakes during the cycle test. Figure 4d and e depict in situ SEM images from the side of a Si thin flake after charging and discharging. The mean thickness increased to approximately 150 nm from approximately 90 nm in the original flakes, and the lithiated Si flakes decreased to approximately 120 nm after the discharge. This irreversible volume change is due to the formation of nanoporous Si by delithiation from the resultant Li-Si alloy26. For reference, low-magnification in situ SEM images obtained during the 3rd cycle are shown in Supplementary Fig. 3a–h. The relevant charge/discharge curve is given in Supplementary Fig. 3i. These SEM images were captured at each point indicated by a-h in the charge/discharge curve.
In addition to the morphology variation in the Si active materials during the charge/discharge process observed by secondary electron (SE) imaging, we also used backscattered electron (BSE) imaging, which can provide dynamic information about elemental distributions. This technique enables the visualization of the lith-iation/delithiation processes of Si materials by means of the composition contrast effect47, i.e., an element with a lower atomic number releases fewer backscattering electrons, thereby generating a dark image. Therefore, the BSE image of Si active materials is dark during the lithiation process because Li incorporates into them. To reveal a clear connection between morphological changes and lithium diffusion, in this investigation, both SE and BSE images were acquired simultaneously (Fig. 5 and Movie 5 and 6). During the charging process, the BSE image was darker because of the lower average atomic weight resulting from the lithiation process, but the brightness returned to its initial state after discharging. Interestingly, the brightness variation in each Si flake occurred uni-formly over a short time, suggesting that quick lithiation/delithiation reactions occurred. Therefore, the remarka-ble charge/discharge characteristics of the Si thin flakes, which have been previously reported10,11, are attributable to their flexible nature and facile lithiation/delithiation kinetics, as visually demonstrated in this study.
Figure 6 illustrates the lithiation process of Si active materials based on in situ SEM. An anode with Si microparticles suffered serious damage by pulverization and a conductive network breakdown at an early stage of lithiation (Fig. 6a). The use of Si nanoparticle aggregates mitigates the mechanical and electrical failures to some extent. However, as shown in Supplementary Fig. 4, the discharge capacity gradually decreased with the cycle number. Si nanoparticles exfoliate from the aggregates because of the insufficient strength of the interfacial bonds among the nanoparticles during continuous electrochemical cycling. Nevertheless, Si nanoparticles themselves have good potential as an anode active material for future LIBs2,4. This lithiation model is depicted in Fig. 6b. As for Si thin flakes, the Li diffusion length from a surface layer to the core is short, and its flexible nature can spon-taneously relieve the stress caused by lithiation/delithiation processes (Fig. 6c). As a result, the Si anode exhibits
Figure 4. In situ SEM images of a Si thin flake anode during charge/discharge processes. (a) The charge/
discharge curves of a Si thin flake anode recorded in constant current and constant voltage (CC/CV) mode with cut-off voltages ranging between − 3.88 V and − 2.40 V (vs. LiCoO2). The CC rates for the charge and discharge were 0.5 C. (b) In situ SEM images taken before and after the 3rd cycle. (c) Schematic drawings of two expansion models during the lithiation process revealed by in situ SEM. (d,e) In situ SEM images of a Si thin flake taken from the side after (d) the charge and (e) discharge processes.
better cyclability. As shown in Supplementary Fig. 4, the LIB cell employing Si thin flakes exhibited a stable dis-charge capacity after the initial few cycles. Furthermore, its retention was twice as high as that of a Si nanoparticle aggregate anode after 10 cycles.
Studying the morphological variations in different types of Si anode active materials in LIB cells during the charge/discharge process is directly related to the rational design of durable and high-capacity Si anodes. In this article, using our established in situ electron microscope techniques, we visually demonstrated that the frac-ture resistance and volume change characteristics of Si active materials show significant size and shape depend-encies. This study revealed that Si thin flakes show an unexpected shape variation that spontaneously relieves the mechanical stress caused during charge/discharge processes. Additionally, the in situ electron microscope approach described here enables the simultaneous recording of three different types of information: electro-chemical data, morphological variation process data, and dynamic information on the elemental distribution during the lithiation/delithiation of Si anode materials. If a SEM system for in situ observation is equipped with an extra X-ray detector, further useful information could be readily obtained to identify electrode reactions and parasitic reactions, including SEI formation, in LIB cells. This novel in situ analytical approach has great potential for emerging as a useful tool for tailoring high-capacity active materials, such as Si and Sn, and designing anodes for various next-generation IL-based energy-storage devices, including LIBs.
Fabrication of Si anodes.Si anodes were prepared by an EPD method as described in ref. 31. The solution used for the Si anode preparation was dry acetone containing 1.0-g L−1 Si active materials, 0.4-g L−1 AB (Strem Chemicals (USA)), and 1.0-g L−1 citric acid monohydrate (Wako (Japan)). The Si active materials used in this
Figure 5. In situ secondary and backscattered electron images of a Si thin flake anode during (a) the 2nd
discharge and (b) the 3rd charge processes. The charge/discharge process was conducted in constant current and constant voltage (CC/CV) mode with cut-off voltages ranging between − 3.88 V and − 2.40 V (vs. LiCoO2). The CC rates for the charge and discharge processes were 0.5 C.
research were Si thin flakes (Si LeafPowder
®(Si-LP), thickness: 100 nm, lateral size: 4–5 μ m, Oike & Co., Ltd., Kyoto (Japan)), Si microparticles (100 mesh, Nilaco Co. (Japan)), and Si nanoparticle aggregates (325 mesh, Rare Metallic Co., LTD. (Japan)). AB was added as a conduction supporting agent for the Si anodes. The solution was sonicated for 10 min prior to use. A platinum plate was used as the cathode, and copper mesh served as the anode. The electrodes were separated by 2 cm in the bath. The voltage difference between the two electrodes was set at 100 V, and the EPD duration was 15–120 sec. All the Si active material-deposited copper mesh electrodes were dried at 353 K under vacuum overnight to strengthen the adhesion of the Si materials.
LIB cells for in situ SEM.The cell was composed of a binder-free handmade Si anode, a LiCoO2 cathode (3.0 mAh cm−2, Piotrek Co., Ltd. (Japan)), and a glass microfibre filter separator (GF/A, Whatman (UK)). The electrolyte was [C2 mim][FSA] (Kanto Chemical Co., Inc. (Japan)) IL containing 1.0-mol L−1 Li[TFSA] (Morita Chemical Industries Co., Ltd. (Japan)). The cell was assembled in an argon-filled glove box (VAC, OMNI-LAB, H2O, O2 < 1 ppm) and immediately placed on a sample holder in the in situ SEM system.
In situ SEM experiments.We converted a conventional SEM system (S-3400N, Hitachi (Japan); VE-8800, Keyence (Japan)) into an in situ system by attaching feed-through terminals to examine the morphological and electrochemical behaviours of the Si anode. Both SE and BSE modes were used for the investigation. For the charge/discharge experiments, the CC/CV and CC modes were employed. The electrochemical experimental conditions were controlled with a potentiostat/galvanostat (VersaSTAT 4, Princeton Applied Research (USA)). All the electrochemical experiments were conducted in the chamber of the in situ SEM system, as described in our previous work30. Ex situ SEM of the Si anode after the charge/discharge experiments was conducted after rinsing with battery-grade DEC (Wako (Japan)) in an argon-filled glove box.
1. Magasinski, A. et al. High-performance lithium-ion anodes using a hierarchical bottom-up approach. Nature Mater. 9, 353–358 (2010).
2. Su, X. et al. Silicon-based nanomaterials for lithium-ion batteries: a review. Adv. Energy Mater. 4, 1300882 (2014).
3. Wu, H. et al. Stable Li-ion battery anodes by in-situ polymerization of conducting hydrogel to conformally coat silicon nanoparticles.
Nat. Commun. 4, 1943 (2013).
4. Kim, H., Seo, M., Park, M. H. & Cho, J. A critical size of silicon nano-anodes for lithium rechargeable batteries. Angew. Chem. Int.
Ed. 49, 2146–2149 (2010).
5. Chan, C. K. et al. High-performance lithium battery anodes using silicon nanowires. Nature Nanotech. 3, 31–35 (2008).
6. Wu, H. et al. Stable cycling of double-walled silicon nanotube battery anodes through solid-electrolyte interphase control. Nature
Nanotech. 7, 309–314 (2012).
7. Graetz, J., Ahn, C. C., Yazami, R. & Fultz, B. Highly reversible lithium storage in nanostructured silicon. Electrochem. Solid State Lett. 6, A194–A197 (2003).
8. Ohara, S., Suzuki, J., Sekine, K. & Takamura, T. A thin film silicon anode for Li-ion batteries having a very large specific capacity and long cycle life. J. Power Sources 136, 303–306 (2004).
9. Jung, M. S. et al. A bendable Li-ion battery with a nano-hairy electrode: direct integration scheme on the polymer substrate. Adv.
Energy Mater. 5, 1400611 (2015).
Figure 6. Schematic illustrations of morphology variation in Si active materials caused by charge/
discharge processes. The Si active materials were (a) Si microparticles, (b) Si nanoparticle aggregates, and (c) Si
21. Key, B. et al. Real-time NMR investigations of structural changes in silicon electrodes for lithium-ion batteries. J. Am. Chem. Soc. 131, 9239–9249 (2009).
22. Liu, D. X. et al. In situ quantification and visualization of lithium transport with neutrons. Angew. Chem. Int. Ed. 53, 9498–9502 (2014).
23. Ebner, M., Marone, F., Stampanoni, M. & Wood, V. Visualization and quantification of electrochemical and mechanical degradation in Li ion batteries. Science 342, 716–720 (2013).
24. Huang, J. Y. et al. In situ observation of the electrochemical lithiation of a single SnO2 nanowire electrode. Science 330, 1515–1520
25. McDowell, M. T. et al. Studying the kinetics of crystalline silicon nanoparticle lithiation with in situ transmission electron microscopy. Adv. Mater. 24, 6034–6041 (2012).
26. Gu, M. et al. In situ TEM study of lithiation behavior of silicon nanoparticles attached to and embedded in a carbon matrix. ACS
Nano 6, 8439–8447 (2012).
27. Arimoto, S., Oyamatsu, D., Torimoto, T. & Kuwabata, S. Development of in situ electrochemical scanning electron microscopy with ionic liquids as electrolytes. ChemPhysChem 9, 763–767 (2008).
28. Nagao, M. et al. In situ SEM study of a lithium deposition and dissolution mechanism in a bulk-type solid-state cell with Li2S–P2S5
solid electrolyte. Phys. Chem. Chem. Phys. 15, 18600–18606 (2013).
29. Tsuda, T. et al. Nonvolatile RTIL-based artificial muscle: actuation mechanism identified by in situ EDX analysis. Chem. Eur. J. 17, 11122–11126 (2011).
30. Tsuda, T. et al. In situ SEM observation of the Si negative electrode reaction in an ionic-liquid-based lithium-ion secondary battery.
Microscopy 64, 159–168 (2015).
31. Yang, Y., Chen, D. Q., Liu, B. & Zhao, J. B. Binder-free Si nanoparticle electrode with 3D porous structure prepared by electrophoretic deposition for lithium-ion batteries. ACS Appl. Mater. Interfaces 7, 7497–7504 (2015).
32. Ishikawa, M., Sugimoto, T., Kikuta, M., Ishiko, E. & Kono, M. Pure ionic liquid electrolytes compatible with a graphitized carbon negative electrode in rechargeable lithium-ion batteries. J. Power Sources 162, 658–662 (2006).
33. Uematsu, T. et al. Atomic resolution imaging of gold nanoparticle generation and growth in ionic liquid. J. Am. Chem. Soc. 136, 13789–13797 (2014).
34. Itoi, M. et al. Direct observation of short-range structural coherence during a charge transfer induced spin transition in a CoFe Prussian blue analogue by transmission electron microscopy. J. Am. Chem. Soc. 137, 14686–14693 (2015).
35. Tsuda, T. et al. Observation of electrochemical reaction and biological specimen by novel analytical technique combined with room-temperature ionic liquid and scanning electron microscope. Electrochemistry 80, 308–311 (2012).
36. Ryu, J. H., Kim, J. W., Sung, Y. E. & Oh, S. M. Failure modes of silicon powder negative electrode in lithium secondary batteries.
Electrochem. Solid-State Lett. 7, A306–A309 (2004).
37. Weker, J. N. et al. In situ nanotomography and operando transmission X-ray microscopy of micron-sized Ge particles. Energy
Environ. Sci. 7, 2771–2777 (2014).
38. Zhao, K. J. et al. Concurrent reaction and plasticity during initial lithiation of crystalline silicon in lithium-ion batteries.
J. Electrochem. Soc. 159, A238–A243 (2012).
39. Liu, X. H. et al. Size-dependent fracture of silicon nanoparticles during lithiation. ACS Nano 6, 1522–1531 (2012).
40. Shkrob, I. A., Marin, T. W., Zhu, Y. & Abraham, D. P. Why bis(fluorosulfonyl)imide is a “magic anion” for electrochemistry. J. Phys.
Chem. C 118, 19661–19671 (2014).
41. Kornyshev, A. A. Double-layer in ionic liquids: paradigm change. J. Phys. Chem. B 111, 5545–5557 (2007).
42. Boukamp, B. A., Lesh, G. C. & Huggins, R. A. All-solid lithium electrodes with mixed-conductor matrix. J. Electrochem. Soc. 128, 725–729 (1981).
43. Kim, H., Chou, C. Y., Ekerdt, J. G. & Hwang, G. S. Structure and properties of Li–Si alloys: a first-principles study. J. Phys. Chem.
C 115, 2514–2521 (2011).
44. Hovington, P. et al. In situ scanning electron microscope study and microstructural evolution of nano silicon anode for high energy Li-ion batteries. J. Power Sources 248, 457–464 (2014).
45. Lee, S. W., McDowell, M. T., Berla, L. A., Nix, W. D. & Cui, Y. Fracture of crystalline silicon nanopillars during electrochemical lithium insertion. Proc. Natl. Acad. Sci. USA 109, 4080–4085 (2012).
46. Kalnaus, S., Rhodes, K. & Daniel, C. A study of lithium ion intercalation induced fracture of silicon particles used as anode material in Li-ion battery. J. Power Sources 196, 8116–8124 (2011).
47. Goldstein, J. et al. Scanning Electron Microscopy and X-Ray Microanalysis (Springer US, 2003).
Part of this research was supported by Grants-in-Aid for Scientific Research (grant numbers 15H03591, 15K13287, and 15H02202) from the Japanese Ministry of Education, Culture, Sports, Science and Technology (MEXT) and by the Advanced Low Carbon Technology Research and Development Program (ALCA) for Specially Promoted Research for Innovative Next Generation Batteries (SPRING), Japan Science and Technology Agency (JST). The silicon thin flakes (Si LeafPowder
®) were provided by Oike & Co., Ltd. (Kyoto, Japan).
T.T. and S.K. planned the research and designed the LIB cell used in this study. T.T., K.U., Y.O., M.Y., M.I., M.H., T.D. and M.I. contributed to the fabrication of the LIB cell. T.S. and C.-Y.C. conducted the experiments. T.T. and C.-Y.C. prepared the manuscript.
Supplementary information accompanies this paper at http://www.nature.com/srep Competing financial interests: The authors declare no competing financial interests.
How to cite this article: Chen, C.-Y. et al. In situ Scanning Electron Microscopy of Silicon Anode Reactions in
Lithium-Ion Batteries during Charge/Discharge Processes. Sci. Rep. 6, 36153; doi: 10.1038/srep36153 (2016).
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/